The second cuprate by practical importance is currently BSCCO, a compound of Bi–Sr–Ca–Cu–O. The content of bismuth and strontium creates some chemical issues. It has three superconducting phases forming a homologous series as Bi 2 Sr 2 Ca n −1 Cu n O 4+2 n + x (n =1, 2 and 3). These three phases are Bi-2201, Bi-2212 and Bi-2223, having transition temperatures of 20 K (−253.2 °C), 85 K (−188.2 °C) and 110 K (−163 °C), respectively, where the numbering system represent number of atoms for Bi Sr, Ca and Cu respectively. The two phases have a tetragonal structure which consists of two sheared crystallographic unit cells. The unit cell of these phases has double Bi–O planes which are stacked in a way that the Bi atom of one plane sits below the oxygen atom of the next consecutive plane. The Ca atom forms a layer within the interior of the CuO 2 layers in both Bi-2212 and Bi-2223; there is no Ca layer in the Bi-2201 phase. The three phases differ with each other in the number of cuprate planes; Bi-2201, Bi-2212 and Bi-2223 phases have one, two and three CuO 2 planes, respectively. The c axis lattice constants of these phases increases with the number of cuprate planes (see table below). The coordination of the Cu atom is different in the three phases. The Cu atom forms an octahedral coordination with respect to oxygen atoms in the 2201 phase, whereas in 2212, the Cu atom is surrounded by five oxygen atoms in a pyramidal arrangement. In the 2223 structure, Cu has two coordinations with respect to oxygen: one Cu atom is bonded with four oxygen atoms in square planar configuration and another Cu atom is coordinated with five oxygen atoms in a pyramidal arrangement.